#------------------------------------------------------------------------------
#$Date: 2019-11-08 00:45:34 +0200 (Fri, 08 Nov 2019) $
#$Revision: 224323 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/87/7048795.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7048795
loop_
_publ_author_name
'Wang, Hai-Dan'
'Wang, Xing-Fang'
'Su, Fang'
'Li, Jian-Sheng'
'Zhang, Lan-Cui'
'Sang, Xiao-Jing'
'Zhu, Zai-Ming'
_publ_section_title
;
 Carboxyethyltin and transition metal co-functionalized tungstoantimonates
 composited with polypyrrole for enhanced electrocatalytic methanol
 oxidation.
;
_journal_issue                   9
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2977
_journal_page_last               2987
_journal_paper_doi               10.1039/c8dt05118f
_journal_volume                  48
_journal_year                    2019
_chemical_formula_moiety         'C6 H9 Mn2 Na9 O70 Sb2 Sn2 W18,24H2O'
_chemical_formula_sum            'C6 H57 Mn2 Na9 O94 Sb2 Sn2 W18'
_chemical_formula_weight         5740.48
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2019-01-28 deposited with the CCDC.
2019-01-29 downloaded from the CCDC.
;
_cell_angle_alpha                93.553(3)
_cell_angle_beta                 110.782(3)
_cell_angle_gamma                99.534(3)
_cell_formula_units_Z            1
_cell_length_a                   12.621(3)
_cell_length_b                   12.751(2)
_cell_length_c                   16.797(3)
_cell_measurement_reflns_used    4512
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      31.09
_cell_measurement_theta_min      1.31
_cell_volume                     2470.9(8)
_computing_cell_refinement       'SMART (Bruker, 2005)'
_computing_data_collection       'SMART (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL (Sheldrick, 1997a)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0288
_diffrn_reflns_av_unetI/netI     0.0554
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            12707
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         1.633
_exptl_absorpt_coefficient_mu    22.280
_exptl_absorpt_correction_T_max  0.3297
_exptl_absorpt_correction_T_min  0.2390
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.858
_exptl_crystal_description       block
_exptl_crystal_F_000             2528
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.072
_exptl_crystal_size_min          0.064
_refine_diff_density_max         3.339
_refine_diff_density_min         -3.285
_refine_diff_density_rms         0.424
_refine_ls_extinction_coef       0.00026(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.031
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     655
_refine_ls_number_reflns         8627
_refine_ls_number_restraints     104
_refine_ls_restrained_S_all      1.032
_refine_ls_R_factor_all          0.0496
_refine_ls_R_factor_gt           0.0417
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0777P)²+4.2258P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1139
_refine_ls_wR_factor_ref         0.1192
_reflns_Friedel_coverage         0.000
_reflns_number_gt                7385
_reflns_number_total             8627
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8dt05118f2.cif
_cod_data_source_block           SbW9-Mn-SnR
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7048795--7048798.cif.
;
_cod_original_cell_volume        2470.8(8)
_cod_database_code               7048795
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.239
_shelx_estimated_absorpt_t_max   0.330
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 1.06305(4) 0.13346(4) -0.09223(3) 0.01215(13) Uani 1 1 d . . . . .
W2 W 0.90689(4) 0.10878(4) -0.30584(3) 0.01586(14) Uani 1 1 d . . . . .
W3 W 0.71972(5) -0.15038(4) -0.42660(4) 0.01910(14) Uani 1 1 d . . . . .
W4 W 1.15002(4) 0.01130(4) -0.23834(4) 0.01677(14) Uani 1 1 d . . . . .
W5 W 0.99437(5) -0.25611(4) -0.35865(4) 0.02007(14) Uani 1 1 d . . . . .
W6 W 0.64795(4) -0.03317(4) -0.27467(3) 0.01715(14) Uani 1 1 d . . . . .
W7 W 0.89244(5) -0.40997(4) -0.23222(4) 0.02083(15) Uani 1 1 d . . . . .
W8 W 1.15476(4) -0.25045(4) -0.15288(4) 0.01864(14) Uani 1 1 d . . . . .
W9 W 0.62862(4) -0.29865(4) -0.29351(4) 0.02170(15) Uani 1 1 d . . . . .
Sb1 Sb 0.90485(7) -0.13257(6) -0.17114(5) 0.01322(19) Uani 1 1 d . . . . .
Sn1 Sn 0.78830(7) 0.07233(6) -0.04090(6) 0.01426(19) Uani 1 1 d . . . . .
Mn1 Mn 0.74982(17) -0.38043(15) -0.07779(14) 0.0205(4) Uani 1 1 d . . . . .
Na1 Na 0.8126(6) 0.2863(5) -0.1919(5) 0.0445(17) Uani 1 1 d . . . . .
Na2 Na 1.3383(6) 0.0064(6) -0.3734(5) 0.0478(17) Uani 1 1 d . . . . .
Na3 Na 1.2808(7) 0.4085(6) -0.2387(7) 0.067(2) Uani 1 1 d . . . . .
Na4 Na 0.7799(12) 0.2420(11) -0.5119(9) 0.046(3) Uani 0.5 1 d . U P . .
Na5 Na 1.1300(17) 0.4291(15) -0.4410(13) 0.080(4) Uani 0.5 1 d . U P . .
Na6 Na 0.6929(17) 0.5540(14) -0.5014(14) 0.082(4) Uani 0.5 1 d . U P . .
O1 O 0.8737(8) 0.2073(7) -0.3704(6) 0.026(2) Uani 1 1 d . . . . .
O2 O 0.7452(8) -0.3774(7) -0.2992(6) 0.026(2) Uani 1 1 d . U . . .
O3 O 1.1420(8) -0.2713(7) -0.2732(6) 0.023(2) Uani 1 1 d . U . . .
O4 O 1.1145(7) 0.0293(7) -0.0277(6) 0.023(2) Uani 1 1 d . . . . .
O5 O 1.0568(8) -0.1051(7) -0.3320(6) 0.022(2) Uani 1 1 d . . . . .
O6 O 0.9227(7) 0.1186(7) -0.0806(6) 0.0195(19) Uani 1 1 d . . . . .
O7 O 0.6210(7) -0.2714(7) -0.4168(6) 0.022(2) Uani 1 1 d . . . . .
O8 O 0.9899(7) 0.2003(6) -0.1993(6) 0.0156(18) Uani 1 1 d . . . . .
O9 O 0.8386(8) -0.0181(7) -0.3876(6) 0.022(2) Uani 1 1 d . . . . .
O10 O 0.8419(8) -0.2263(7) -0.4127(6) 0.023(2) Uani 1 1 d . . . . .
O11 O 0.6797(8) -0.2895(8) -0.1799(7) 0.030(2) Uani 1 1 d . . . . .
O12 O 0.6694(8) -0.1510(8) -0.5365(7) 0.030(2) Uani 1 1 d . . . . .
O13 O 0.9831(7) -0.0021(6) -0.2046(6) 0.0156(18) Uani 1 1 d . . . . .
O14 O 0.7630(7) -0.1511(6) -0.2806(6) 0.0170(18) Uani 1 1 d . . . . .
O15 O 0.9689(7) -0.2340(6) -0.2305(6) 0.0189(19) Uani 1 1 d . . . . .
O16 O 1.1904(8) -0.0966(7) -0.1689(6) 0.024(2) Uani 1 1 d . . . . .
O17 O 0.7730(7) 0.0782(6) -0.2751(6) 0.0165(18) Uani 1 1 d . . . . .
O18 O 0.5529(7) -0.1749(7) -0.2953(6) 0.0203(19) Uani 1 1 d . . . . .
O19 O 0.6249(7) -0.0598(7) -0.3992(6) 0.0203(19) Uani 1 1 d . U . . .
O20 O 0.8793(8) -0.3734(8) -0.1337(7) 0.028(2) Uani 1 1 d . . . . .
O21 O 1.0654(8) -0.3911(7) -0.1713(6) 0.023(2) Uani 1 1 d . . . . .
O22 O 1.1222(7) -0.1989(7) -0.0617(6) 0.021(2) Uani 1 1 d . U . . .
O23 O 0.7198(7) -0.0318(6) -0.1601(6) 0.0186(19) Uani 1 1 d . . . . .
O24 O 1.1435(7) 0.2504(7) -0.0264(6) 0.023(2) Uani 1 1 d . . . . .
O25 O 1.0254(10) -0.2854(8) -0.4487(7) 0.035(2) Uani 1 1 d . . . . .
O26 O 0.9314(8) -0.3951(7) -0.3400(6) 0.025(2) Uani 1 1 d . . . . .
O27 O 0.5055(9) -0.4004(9) -0.3283(8) 0.043(3) Uani 1 1 d . . . . .
O28 O 1.2705(8) 0.0481(8) -0.2658(7) 0.029(2) Uani 1 1 d . . . . .
O29 O 0.5412(7) 0.0406(7) -0.2858(6) 0.023(2) Uani 1 1 d . . . . .
O30 O 1.2949(9) -0.2721(9) -0.1040(8) 0.042(3) Uani 1 1 d . . . . .
O31 O 1.0534(8) 0.0977(7) -0.3140(6) 0.0190(19) Uani 1 1 d . . . . .
O32 O 0.8665(9) -0.5496(7) -0.2452(8) 0.038(3) Uani 1 1 d . . . . .
O33 O 1.1816(7) 0.1184(7) -0.1465(6) 0.020(2) Uani 1 1 d . . . . .
O34 O 0.7113(7) 0.1968(7) -0.1109(6) 0.023(2) Uani 1 1 d . . . . .
O35 O 0.5573(9) 0.2718(9) -0.1400(9) 0.044(3) Uani 1 1 d . . . . .
C1 C 0.6255(10) 0.0347(10) -0.0251(9) 0.019(3) Uani 1 1 d . . . . .
H1A H 0.5913 -0.0408 -0.0439 0.023 Uiso 1 1 calc R U . . .
H1B H 0.6362 0.0503 0.0348 0.023 Uiso 1 1 calc R U . . .
C2 C 0.5466(11) 0.1039(11) -0.0799(10) 0.026(3) Uani 1 1 d . U . . .
H2A H 0.5071 0.1332 -0.0463 0.031 Uiso 1 1 calc R U . . .
H2B H 0.4881 0.0578 -0.1293 0.031 Uiso 1 1 calc R U . . .
C3 C 0.6082(12) 0.1993(11) -0.1131(10) 0.027(3) Uani 1 1 d . . . . .
O1W O 0.6533(15) -0.5324(10) -0.1660(10) 0.069(4) Uani 1 1 d D . . . .
H1WA H 0.592(10) -0.521(12) -0.160(15) 0.083 Uiso 1 1 d D U . . .
H1WB H 0.657(15) -0.597(6) -0.157(14) 0.083 Uiso 1 1 d D U . . .
O2W O 0.8351(12) -0.4844(10) 0.0147(8) 0.048(3) Uani 1 1 d D . . . .
H2WA H 0.855(16) -0.468(12) 0.069(2) 0.058 Uiso 1 1 d D U . . .
H2WB H 0.856(14) -0.543(7) 0.008(9) 0.058 Uiso 1 1 d D U . . .
O3W O 0.6131(11) -0.3844(13) -0.0292(11) 0.064(4) Uani 1 1 d D . . . .
H3WA H 0.564(14) -0.438(10) -0.062(8) 0.077 Uiso 1 1 d D U . . .
H3WB H 0.627(17) -0.397(14) 0.022(3) 0.077 Uiso 1 1 d D U . . .
O4W O 0.9243(9) 0.3646(8) -0.0427(7) 0.035(3) Uani 1 1 d D . . . .
H4WA H 0.944(10) 0.333(10) 0.002(6) 0.042 Uiso 1 1 d D U . . .
H4WB H 0.986(6) 0.403(10) -0.043(9) 0.042 Uiso 1 1 d D U . . .
O5W O 1.3797(10) -0.0979(11) -0.4887(8) 0.053(3) Uani 1 1 d D . . . .
H5WA H 1.370(15) -0.068(11) -0.534(6) 0.063 Uiso 1 1 d D U . . .
H5WB H 1.415(14) -0.148(9) -0.493(10) 0.063 Uiso 1 1 d D U . . .
O6W O 1.3512(10) 0.2935(9) -0.1319(10) 0.051(4) Uani 1 1 d D . . . .
H6WA H 1.330(14) 0.258(10) -0.097(8) 0.061 Uiso 1 1 d D U . . .
H6WB H 1.385(12) 0.254(9) -0.153(9) 0.061 Uiso 1 1 d D U . . .
O7W O 1.3143(10) -0.1856(12) -0.3410(9) 0.030(3) Uani 0.75 1 d . . P . .
O8W O 1.1235(11) 0.4015(10) -0.1946(11) 0.037(4) Uani 0.75 1 d . . P . .
O9W O 1.1478(15) -0.0564(13) -0.4611(12) 0.021(4) Uani 0.5 1 d . U P . .
O10W O 1.1689(15) 0.2647(13) -0.3704(12) 0.021(4) Uiso 0.5 1 d . . P A .
O11W O 0.6296(15) 0.2687(13) -0.3149(12) 0.021(4) Uiso 0.5 1 d . . P . .
O12W O 1.3844(18) 0.5428(16) -0.0991(15) 0.037(5) Uiso 0.5 1 d . . P . .
O13W O 1.417(2) 0.3722(19) -0.3138(17) 0.051(6) Uiso 0.5 1 d . . P . .
O14W O 1.245(3) 0.554(3) -0.319(2) 0.085(10) Uiso 0.5 1 d . . P A .
O15W O 0.625(2) 0.339(2) -0.4755(19) 0.061(4) Uiso 0.5 1 d . U P A .
O16W O 0.978(2) 0.415(2) -0.397(2) 0.061(4) Uiso 0.5 1 d . U P A 1
O17W O 0.896(3) 0.431(2) -0.461(2) 0.066(3) Uiso 0.5 1 d . U P A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O24 W1 O4 103.1(4) . .
O24 W1 O6 104.2(4) . .
O4 W1 O6 96.7(4) . .
O24 W1 O8 97.5(4) . .
O4 W1 O8 157.7(4) . .
O6 W1 O8 86.2(4) . .
O24 W1 O33 94.5(4) . .
O4 W1 O33 87.5(4) . .
O6 W1 O33 159.3(4) . .
O8 W1 O33 82.5(4) . .
O24 W1 O13 163.3(4) . .
O4 W1 O13 85.3(4) . .
O6 W1 O13 88.8(3) . .
O8 W1 O13 72.7(3) . .
O33 W1 O13 71.3(3) . .
O1 W2 O9 101.4(4) . .
O1 W2 O8 97.8(4) . .
O9 W2 O8 160.8(4) . .
O1 W2 O17 101.5(4) . .
O9 W2 O17 86.5(4) . .
O8 W2 O17 90.3(3) . .
O1 W2 O31 98.8(4) . .
O9 W2 O31 88.0(4) . .
O8 W2 O31 88.5(4) . .
O17 W2 O31 159.7(4) . .
O1 W2 O13 169.5(4) . .
O9 W2 O13 87.2(4) . .
O8 W2 O13 73.7(3) . .
O17 W2 O13 84.9(3) . .
O31 W2 O13 75.3(3) . .
O1 W2 Na1 75.5(3) . .
O9 W2 Na1 136.8(3) . .
O8 W2 Na1 49.8(3) . .
O17 W2 Na1 53.3(2) . .
O31 W2 Na1 135.2(3) . .
O13 W2 Na1 102.4(2) . .
O12 W3 O7 101.1(4) . .
O12 W3 O10 99.6(4) . .
O7 W3 O10 92.4(4) . .
O12 W3 O19 99.0(4) . .
O7 W3 O19 89.6(4) . .
O10 W3 O19 160.4(4) . .
O12 W3 O9 101.4(4) . .
O7 W3 O9 157.2(4) . .
O10 W3 O9 87.3(4) . .
O19 W3 O9 83.4(4) . .
O12 W3 O14 172.7(4) . .
O7 W3 O14 74.5(3) . .
O10 W3 O14 86.5(4) . .
O19 W3 O14 75.4(3) . .
O9 W3 O14 82.8(3) . .
O28 W4 O16 102.7(4) . .
O28 W4 O33 100.8(4) . .
O16 W4 O33 95.1(4) . .
O28 W4 O31 96.4(4) . .
O16 W4 O31 159.6(4) . .
O33 W4 O31 88.3(4) . .
O28 W4 O5 100.7(4) . .
O16 W4 O5 86.7(4) . .
O33 W4 O5 157.5(3) . .
O31 W4 O5 82.7(4) . .
O28 W4 O13 168.3(4) . .
O16 W4 O13 87.6(3) . .
O33 W4 O13 72.5(3) . .
O31 W4 O13 74.2(3) . .
O5 W4 O13 85.2(3) . .
O25 W5 O26 102.0(4) . .
O25 W5 O5 100.7(4) . .
O26 W5 O5 156.8(4) . .
O25 W5 O10 99.7(5) . .
O26 W5 O10 91.4(4) . .
O5 W5 O10 89.5(4) . .
O25 W5 O3 97.2(5) . .
O26 W5 O3 87.0(4) . .
O5 W5 O3 85.3(4) . .
O10 W5 O3 163.0(4) . .
O25 W5 O15 171.9(4) . .
O26 W5 O15 73.5(3) . .
O5 W5 O15 83.4(3) . .
O10 W5 O15 87.2(4) . .
O3 W5 O15 76.1(3) . .
O25 W5 Na5 40.7(5) . 2_754
O26 W5 Na5 70.8(4) . 2_754
O5 W5 Na5 131.5(4) . 2_754
O10 W5 Na5 75.0(4) . 2_754
O3 W5 Na5 120.1(4) . 2_754
O15 W5 Na5 139.4(4) . 2_754
O29 W6 O23 105.5(4) . .
O29 W6 O18 98.3(4) . .
O23 W6 O18 96.0(4) . .
O29 W6 O17 100.3(4) . .
O23 W6 O17 90.3(4) . .
O18 W6 O17 158.0(3) . .
O29 W6 O19 97.7(4) . .
O23 W6 O19 156.4(4) . .
O18 W6 O19 84.6(4) . .
O17 W6 O19 81.3(4) . .
O29 W6 O14 169.5(4) . .
O23 W6 O14 82.5(3) . .
O18 W6 O14 73.7(3) . .
O17 W6 O14 86.4(3) . .
O19 W6 O14 75.1(3) . .
O32 W7 O20 104.9(5) . .
O32 W7 O2 103.8(5) . .
O20 W7 O2 93.2(4) . .
O32 W7 O21 95.0(4) . .
O20 W7 O21 89.9(4) . .
O2 W7 O21 159.4(4) . .
O32 W7 O26 95.1(4) . .
O20 W7 O26 159.5(4) . .
O2 W7 O26 85.8(4) . .
O21 W7 O26 84.2(4) . .
O32 W7 O15 162.7(4) . .
O20 W7 O15 88.2(4) . .
O2 W7 O15 86.2(4) . .
O21 W7 O15 73.5(3) . .
O26 W7 O15 71.3(3) . .
O30 W8 O22 102.9(5) . .
O30 W8 O21 101.7(5) . .
O22 W8 O21 97.2(4) . .
O30 W8 O3 98.5(5) . .
O22 W8 O3 156.4(4) . .
O21 W8 O3 88.0(4) . .
O30 W8 O16 99.7(5) . .
O22 W8 O16 85.0(4) . .
O21 W8 O16 157.3(4) . .
O3 W8 O16 81.7(4) . .
O30 W8 O15 173.6(4) . .
O22 W8 O15 83.3(4) . .
O21 W8 O15 75.4(3) . .
O3 W8 O15 75.8(3) . .
O16 W8 O15 82.5(3) . .
O27 W9 O11 104.2(5) . .
O27 W9 O2 101.3(5) . .
O11 W9 O2 92.1(4) . .
O27 W9 O18 98.4(5) . .
O11 W9 O18 92.8(4) . .
O2 W9 O18 157.8(4) . .
O27 W9 O7 95.3(5) . .
O11 W9 O7 160.4(4) . .
O2 W9 O7 82.1(4) . .
O18 W9 O7 86.1(4) . .
O27 W9 O14 165.0(5) . .
O11 W9 O14 89.0(4) . .
O2 W9 O14 85.1(3) . .
O18 W9 O14 73.4(3) . .
O7 W9 O14 71.9(3) . .
O13 Sb1 O15 93.3(3) . .
O13 Sb1 O14 91.8(3) . .
O15 Sb1 O14 89.0(4) . .
O6 Sn1 O4 86.0(4) . 2_755
O6 Sn1 O22 84.9(3) . 2_755
O4 Sn1 O22 89.9(4) 2_755 2_755
O6 Sn1 O23 82.6(3) . .
O4 Sn1 O23 95.3(4) 2_755 .
O22 Sn1 O23 166.1(3) 2_755 .
O6 Sn1 C1 167.5(5) . .
O4 Sn1 C1 105.2(4) 2_755 .
O22 Sn1 C1 100.4(4) 2_755 .
O23 Sn1 C1 90.7(4) . .
O6 Sn1 O34 86.1(3) . .
O4 Sn1 O34 170.9(3) 2_755 .
O22 Sn1 O34 84.9(4) 2_755 .
O23 Sn1 O34 88.2(3) . .
C1 Sn1 O34 83.2(4) . .
O11 Mn1 O20 80.7(4) . .
O11 Mn1 O3W 95.8(5) . .
O20 Mn1 O3W 176.3(5) . .
O11 Mn1 O24 100.6(4) . 2_755
O20 Mn1 O24 93.0(4) . 2_755
O3W Mn1 O24 88.7(5) . 2_755
O11 Mn1 O2W 171.1(5) . .
O20 Mn1 O2W 91.3(5) . .
O3W Mn1 O2W 92.2(6) . .
O24 Mn1 O2W 83.6(4) 2_755 .
O11 Mn1 O1W 89.8(5) . .
O20 Mn1 O1W 88.6(5) . .
O3W Mn1 O1W 90.4(6) . .
O24 Mn1 O1W 169.6(5) 2_755 .
O2W Mn1 O1W 86.1(6) . .
O34 Na1 O32 147.5(5) . 1_565
O34 Na1 O4W 75.2(4) . .
O32 Na1 O4W 92.2(4) 1_565 .
O34 Na1 O11W 90.4(5) . .
O32 Na1 O11W 83.7(5) 1_565 .
O4W Na1 O11W 145.9(6) . .
O34 Na1 O8 114.2(4) . .
O32 Na1 O8 95.5(4) 1_565 .
O4W Na1 O8 91.0(4) . .
O11W Na1 O8 123.1(5) . .
O34 Na1 O17 82.8(3) . .
O32 Na1 O17 125.8(4) 1_565 .
O4W Na1 O17 131.2(4) . .
O11W Na1 O17 75.4(5) . .
O8 Na1 O17 59.4(3) . .
O34 Na1 W2 112.4(3) . .
O32 Na1 W2 99.6(3) 1_565 .
O4W Na1 W2 123.2(4) . .
O11W Na1 W2 90.8(4) . .
O8 Na1 W2 33.01(19) . .
O17 Na1 W2 33.38(18) . .
O9W Na2 O28 86.8(5) . .
O9W Na2 O29 170.1(6) . 1_655
O28 Na2 O29 97.8(4) . 1_655
O9W Na2 O12 85.3(5) . 2_754
O28 Na2 O12 110.1(4) . 2_754
O29 Na2 O12 101.2(4) 1_655 2_754
O9W Na2 O7W 80.3(5) . .
O28 Na2 O7W 87.7(4) . .
O29 Na2 O7W 91.1(4) 1_655 .
O12 Na2 O7W 156.5(5) 2_754 .
O9W Na2 O5W 84.0(6) . .
O28 Na2 O5W 161.8(5) . .
O29 Na2 O5W 89.1(4) 1_655 .
O12 Na2 O5W 84.8(4) 2_754 .
O7W Na2 O5W 75.3(4) . .
O9W Na2 Na4 53.2(5) . 2_754
O28 Na2 Na4 115.5(4) . 2_754
O29 Na2 Na4 116.9(4) 1_655 2_754
O12 Na2 Na4 113.4(4) 2_754 2_754
O7W Na2 Na4 43.2(4) . 2_754
O5W Na2 Na4 46.9(4) . 2_754
O8W Na3 O14W 96.2(9) . .
O8W Na3 O6W 86.6(5) . .
O14W Na3 O6W 166.3(10) . .
O8W Na3 O13W 164.7(8) . .
O14W Na3 O13W 87.6(10) . .
O6W Na3 O13W 93.1(7) . .
O8W Na3 O10W 93.9(6) . .
O14W Na3 O10W 93.8(10) . .
O6W Na3 O10W 99.3(6) . .
O13W Na3 O10W 71.0(7) . .
O8W Na3 O12W 82.3(7) . .
O14W Na3 O12W 89.8(10) . .
O6W Na3 O12W 77.3(6) . .
O13W Na3 O12W 112.6(8) . .
O10W Na3 O12W 175.0(7) . .
O8W Na3 Na5 94.6(6) . .
O14W Na3 Na5 45.5(9) . .
O6W Na3 Na5 147.8(6) . .
O13W Na3 Na5 77.5(7) . .
O10W Na3 Na5 48.5(6) . .
O12W Na3 Na5 134.8(7) . .
O7W Na4 O1 151.4(8) 2_754 .
O7W Na4 O5W 79.7(6) 2_754 2_754
O1 Na4 O5W 83.8(5) . 2_754
O7W Na4 O17W 119.3(10) 2_754 .
O1 Na4 O17W 86.1(9) . .
O5W Na4 O17W 149.2(10) 2_754 .
O7W Na4 O15W 101.9(9) 2_754 .
O1 Na4 O15W 95.1(8) . .
O5W Na4 O15W 72.6(7) 2_754 .
O17W Na4 O15W 79.5(9) . .
O7W Na4 O9W 75.5(7) 2_754 2_754
O1 Na4 O9W 78.1(6) . 2_754
O5W Na4 O9W 76.3(6) 2_754 2_754
O17W Na4 O9W 129.5(9) . 2_754
O15W Na4 O9W 148.8(8) . 2_754
O7W Na4 O25 84.2(6) 2_754 2_754
O1 Na4 O25 96.5(6) . 2_754
O5W Na4 O25 144.9(7) 2_754 2_754
O17W Na4 O25 65.2(7) . 2_754
O15W Na4 O25 141.7(8) . 2_754
O9W Na4 O25 69.5(5) 2_754 2_754
O7W Na4 O16W 137.3(8) 2_754 .
O1 Na4 O16W 63.8(7) . .
O5W Na4 O16W 142.8(9) 2_754 .
O15W Na4 O16W 91.7(9) . .
O9W Na4 O16W 111.5(8) 2_754 .
O25 Na4 O16W 61.8(6) 2_754 .
O7W Na4 Na2 48.0(4) 2_754 2_754
O1 Na4 Na2 104.1(5) . 2_754
O5W Na4 Na2 47.9(4) 2_754 2_754
O17W Na4 Na2 162.4(9) . 2_754
O15W Na4 Na2 113.3(7) . 2_754
O9W Na4 Na2 42.2(4) 2_754 2_754
O25 Na4 Na2 99.0(5) 2_754 2_754
O16W Na4 Na2 153.7(8) . 2_754
O16W Na5 O14W 90.7(13) . .
O14W Na5 O17W 93.2(13) . 2_764
O16W Na5 O10W 85.4(11) . .
O14W Na5 O10W 96.1(12) . .
O17W Na5 O10W 165.6(12) 2_764 .
O16W Na5 O25 75.9(9) . 2_754
O14W Na5 O25 166.0(13) . 2_754
O17W Na5 O25 94.1(10) 2_764 2_754
O10W Na5 O25 79.2(7) . 2_754
O16W Na5 Na6 178.2(13) . 2_764
O14W Na5 Na6 90.7(11) . 2_764
O17W Na5 Na6 73.4(9) 2_764 2_764
O10W Na5 Na6 95.5(9) . 2_764
O25 Na5 Na6 102.8(8) 2_754 2_764
O14W Na5 O17W 105.8(12) . .
O17W Na5 O17W 84.3(11) 2_764 .
O10W Na5 O17W 103.5(10) . .
O25 Na5 O17W 63.2(8) 2_754 .
Na6 Na5 O17W 153.1(11) 2_764 .
O16W Na5 Na3 84.3(10) . .
O14W Na5 Na3 45.7(10) . .
O17W Na5 Na3 138.5(10) 2_764 .
O10W Na5 Na3 50.5(6) . .
O25 Na5 Na3 127.3(8) 2_754 .
Na6 Na5 Na3 97.4(7) 2_764 .
O17W Na5 Na3 109.3(9) . .
O16W Na5 W5 101.6(10) . 2_754
O14W Na5 W5 167.6(11) . 2_754
O17W Na5 W5 81.6(9) 2_764 2_754
O10W Na5 W5 87.0(7) . 2_754
O25 Na5 W5 26.3(3) 2_754 2_754
Na6 Na5 W5 77.0(6) 2_764 2_754
O17W Na5 W5 85.0(8) . 2_754
Na3 Na5 W5 136.9(6) . 2_754
O16W Na5 Na5 61.0(9) . 2_764
O14W Na5 Na5 103.4(12) . 2_764
O17W Na5 Na5 45.8(8) 2_764 2_764
O10W Na5 Na5 140.8(10) . 2_764
O25 Na5 Na5 73.7(7) 2_754 2_764
Na6 Na5 Na5 117.6(10) 2_764 2_764
O17W Na5 Na5 38.5(7) . 2_764
Na3 Na5 Na5 135.0(9) . 2_764
W5 Na5 Na5 81.2(6) 2_754 2_764
Na5 Na6 O15W 110.5(9) 2_764 .
Na5 Na6 O7 128.2(8) 2_764 1_565
O15W Na6 O7 118.3(9) . 1_565
W2 O1 Na4 144.9(6) . .
W7 O2 W9 143.3(5) . .
W5 O3 W8 115.5(4) . .
W1 O4 Sn1 165.2(5) . 2_755
W5 O5 W4 144.4(5) . .
W1 O6 Sn1 162.4(5) . .
W3 O7 W9 117.7(4) . .
W3 O7 Na6 100.8(5) . 1_545
W9 O7 Na6 112.1(5) . 1_545
W2 O8 W1 118.9(4) . .
W2 O8 Na1 97.2(4) . .
W1 O8 Na1 111.5(4) . .
W2 O9 W3 146.6(5) . .
W3 O10 W5 155.9(5) . .
W9 O11 Mn1 141.0(5) . .
W3 O12 Na2 132.3(5) . 2_754
Sb1 O13 W1 111.1(4) . .
Sb1 O13 W2 130.4(4) . .
W1 O13 W2 94.6(3) . .
Sb1 O13 W4 125.8(4) . .
W1 O13 W4 94.8(3) . .
W2 O13 W4 91.5(3) . .
Sb1 O14 W9 113.0(4) . .
Sb1 O14 W6 112.1(4) . .
W9 O14 W6 94.9(3) . .
Sb1 O14 W3 138.5(4) . .
W9 O14 W3 95.8(3) . .
W6 O14 W3 93.4(3) . .
Sb1 O15 W7 112.6(4) . .
Sb1 O15 W5 137.5(4) . .
W7 O15 W5 96.3(3) . .
Sb1 O15 W8 114.8(4) . .
W7 O15 W8 93.7(3) . .
W5 O15 W8 92.5(3) . .
W4 O16 W8 147.2(5) . .
W2 O17 W6 145.1(4) . .
W2 O17 Na1 93.3(3) . .
W6 O17 Na1 121.3(4) . .
W6 O18 W9 117.6(4) . .
W3 O19 W6 115.9(4) . .
W7 O20 Mn1 140.1(5) . .
W8 O21 W7 117.2(4) . .
W8 O22 Sn1 132.6(4) . 2_755
W6 O23 Sn1 142.2(5) . .
W1 O24 Mn1 168.9(6) . 2_755
W5 O25 Na5 112.9(7) . 2_754
W5 O25 Na4 134.5(6) . 2_754
Na5 O25 Na4 111.4(6) 2_754 2_754
W5 O26 W7 118.9(4) . .
W4 O28 Na2 140.0(6) . .
W6 O29 Na2 132.7(5) . 1_455
W2 O31 W4 119.0(4) . .
W7 O32 Na1 147.9(7) . 1_545
W4 O33 W1 121.4(4) . .
C3 O34 Sn1 114.1(8) . .
C3 O34 Na1 128.8(9) . .
Sn1 O34 Na1 116.0(4) . .
C2 C1 Sn1 107.3(8) . .
C2 C1 H1A 110.3 . .
Sn1 C1 H1A 110.3 . .
C2 C1 H1B 110.3 . .
Sn1 C1 H1B 110.3 . .
H1A C1 H1B 108.5 . .
C1 C2 C3 116.0(10) . .
C1 C2 H2A 108.3 . .
C3 C2 H2A 108.3 . .
C1 C2 H2B 108.3 . .
C3 C2 H2B 108.3 . .
H2A C2 H2B 107.4 . .
O35 C3 O34 123.2(13) . .
O35 C3 C2 119.5(12) . .
O34 C3 C2 117.4(11) . .
Mn1 O1W H1WA 89(10) . .
Mn1 O1W H1WB 129(10) . .
H1WA O1W H1WB 105.9(17) . .
Mn1 O2W H2WA 122(10) . .
Mn1 O2W H2WB 132(10) . .
H2WA O2W H2WB 106.2(18) . .
Mn1 O3W H3WA 101(10) . .
Mn1 O3W H3WB 118(10) . .
H3WA O3W H3WB 106.8(18) . .
Na1 O4W H4WA 129(10) . .
Na1 O4W H4WB 106(10) . .
H4WA O4W H4WB 106.4(18) . .
Na4 O5W Na2 85.3(5) 2_754 .
Na4 O5W H5WA 118(10) 2_754 .
Na2 O5W H5WA 114(10) . .
Na4 O5W H5WB 87(10) 2_754 .
Na2 O5W H5WB 139(10) . .
H5WA O5W H5WB 106.0(18) . .
Na3 O6W H6WA 140(10) . .
Na3 O6W H6WB 105(10) . .
H6WA O6W H6WB 106.0(17) . .
Na4 O7W Na2 88.8(6) 2_754 .
Na2 O9W Na4 84.5(6) . 2_754
Na5 O10W Na3 81.0(7) . .
Na5 O14W Na3 88.8(12) . .
Na4 O15W Na6 101.9(10) . .
Na5 O16W Na4 110.8(12) . .
Na5 O17W Na4 120.9(14) 2_764 .
Na5 O17W Na5 95.7(11) 2_764 .
Na4 O17W Na5 108.2(11) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O24 1.725(9) .
W1 O4 1.823(9) .
W1 O6 1.831(8) .
W1 O8 2.020(9) .
W1 O33 2.036(8) .
W1 O13 2.288(8) .
W2 O1 1.718(9) .
W2 O9 1.915(9) .
W2 O8 1.916(8) .
W2 O17 1.923(8) .
W2 O31 1.928(9) .
W2 O13 2.324(9) .
W2 Na1 3.489(7) .
W3 O12 1.726(10) .
W3 O7 1.871(8) .
W3 O10 1.907(9) .
W3 O19 1.939(9) .
W3 O9 1.963(8) .
W3 O14 2.316(9) .
W4 O28 1.741(9) .
W4 O16 1.877(10) .
W4 O33 1.878(9) .
W4 O31 1.959(9) .
W4 O5 1.970(9) .
W4 O13 2.351(8) .
W5 O25 1.726(10) .
W5 O26 1.911(9) .
W5 O5 1.915(9) .
W5 O10 1.928(9) .
W5 O3 1.957(10) .
W5 O15 2.294(9) .
W5 Na5 3.583(19) 2_754
W6 O29 1.732(8) .
W6 O23 1.810(9) .
W6 O18 1.932(9) .
W6 O17 1.943(7) .
W6 O19 2.006(9) .
W6 O14 2.277(8) .
W7 O32 1.742(9) .
W7 O20 1.762(10) .
W7 O2 1.929(9) .
W7 O21 2.020(9) .
W7 O26 2.050(10) .
W7 O15 2.285(8) .
W8 O30 1.743(10) .
W8 O22 1.832(9) .
W8 O21 1.897(9) .
W8 O3 1.967(9) .
W8 O16 1.996(9) .
W8 O15 2.296(9) .
W9 O27 1.741(10) .
W9 O11 1.774(10) .
W9 O2 1.939(10) .
W9 O18 1.972(9) .
W9 O7 2.092(9) .
W9 O14 2.257(8) .
Sb1 O13 2.007(8) .
Sb1 O15 2.019(8) .
Sb1 O14 2.028(8) .
Sn1 O6 2.046(8) .
Sn1 O4 2.054(9) 2_755
Sn1 O22 2.126(8) 2_755
Sn1 O23 2.141(9) .
Sn1 C1 2.145(11) .
Sn1 O34 2.185(9) .
Mn1 O11 2.139(11) .
Mn1 O20 2.148(9) .
Mn1 O3W 2.150(12) .
Mn1 O24 2.203(9) 2_755
Mn1 O2W 2.207(12) .
Mn1 O1W 2.240(13) .
Na1 O34 2.394(11) .
Na1 O32 2.415(12) 1_565
Na1 O4W 2.445(13) .
Na1 O11W 2.46(2) .
Na1 O8 2.687(11) .
Na1 O17 2.802(10) .
Na2 O9W 2.301(19) .
Na2 O28 2.326(12) .
Na2 O29 2.405(11) 1_655
Na2 O12 2.448(12) 2_754
Na2 O7W 2.534(16) .
Na2 O5W 2.535(16) .
Na2 Na4 3.408(15) 2_754
Na3 O8W 2.343(15) .
Na3 O14W 2.37(4) .
Na3 O6W 2.404(17) .
Na3 O13W 2.54(3) .
Na3 O10W 2.58(2) .
Na3 O12W 2.59(2) .
Na3 Na5 3.31(2) .
Na4 O7W 2.33(2) 2_754
Na4 O1 2.356(17) .
Na4 O5W 2.495(17) 2_754
Na4 O17W 2.52(3) .
Na4 O15W 2.70(3) .
Na4 O9W 2.74(2) 2_754
Na4 O25 2.744(17) 2_754
Na4 O16W 3.01(3) .
Na4 Na2 3.408(15) 2_754
Na5 O16W 2.27(3) .
Na5 O14W 2.36(4) .
Na5 O17W 2.48(4) 2_764
Na5 O10W 2.51(3) .
Na5 O25 2.54(2) 2_754
Na5 Na6 2.72(3) 2_764
Na5 O17W 2.86(3) .
Na5 W5 3.583(19) 2_754
Na5 Na5 3.97(4) 2_764
Na6 Na5 2.72(3) 2_764
Na6 O15W 2.84(3) .
Na6 O7 3.00(2) 1_565
O4 Sn1 2.054(9) 2_755
O7 Na6 3.00(2) 1_545
O12 Na2 2.449(12) 2_754
O22 Sn1 2.126(8) 2_755
O24 Mn1 2.203(9) 2_755
O25 Na5 2.54(2) 2_754
O25 Na4 2.743(17) 2_754
O29 Na2 2.405(11) 1_455
O32 Na1 2.415(12) 1_545
O34 C3 1.295(15) .
O35 C3 1.230(17) .
C1 C2 1.536(18) .
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 C3 1.572(19) .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
O1W H1WA 0.852(10) .
O1W H1WB 0.852(10) .
O2W H2WA 0.850(10) .
O2W H2WB 0.850(10) .
O3W H3WA 0.848(10) .
O3W H3WB 0.848(10) .
O4W H4WA 0.850(10) .
O4W H4WB 0.849(10) .
O5W Na4 2.495(17) 2_754
O5W H5WA 0.851(10) .
O5W H5WB 0.851(10) .
O6W H6WA 0.851(10) .
O6W H6WB 0.851(10) .
O7W Na4 2.33(2) 2_754
O9W Na4 2.74(2) 2_754
O17W Na5 2.48(4) 2_764
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O1W H1WB O35 0.852(10) 2.02(11) 2.720(16) 139(14) 1_545
O1W H1WA O3W 0.852(10) 2.62(19) 3.12(2) 118(17) .
O2W H2WA O21 0.850(10) 2.64(12) 3.138(15) 119(11) 2_745
O2W H2WA O8W 0.850(10) 2.14(4) 2.97(2) 166(14) 2_755
O2W H2WB O4W 0.850(10) 1.89(7) 2.678(17) 153(15) 1_545
O3W H3WA O12W 0.848(10) 2.09(18) 2.67(2) 125(18) 1_445
O3W H3WB O6W 0.848(10) 2.10(15) 2.73(2) 130(17) 2_755
O3W H3WB O12W 0.848(10) 2.34(12) 3.04(3) 140(15) 2_755
O4W H4WB O2W 0.849(10) 2.19(4) 3.023(17) 166(11) 2_755
O4W H4WA O20 0.850(10) 2.47(9) 3.098(15) 131(10) 2_755
O4W H4WA O22 0.850(10) 2.23(7) 2.944(14) 142(11) 2_755
O5W H5WA O19 0.851(10) 2.04(7) 2.832(15) 155(15) 2_754
O5W H5WB O19 0.851(10) 2.57(17) 2.860(14) 102(13) 1_655
O5W H5WB O15W 0.851(10) 2.39(12) 3.08(3) 139(15) 2_754
O6W H6WA O33 0.851(10) 2.23(15) 2.757(13) 120(14) .
O6W H6WB O35 0.851(10) 2.08(12) 2.711(14) 131(14) 1_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O9 W2 O1 Na4 1.1(11) . .
O8 W2 O1 Na4 -179.6(10) . .
O17 W2 O1 Na4 -87.6(11) . .
O31 W2 O1 Na4 90.8(10) . .
O13 W2 O1 Na4 145.8(17) . .
Na1 W2 O1 Na4 -134.6(11) . .
O24 W1 O4 Sn1 -65(2) . 2_755
O6 W1 O4 Sn1 -172(2) . 2_755
O8 W1 O4 Sn1 92(2) . 2_755
O33 W1 O4 Sn1 29(2) . 2_755
O13 W1 O4 Sn1 100(2) . 2_755
O24 W1 O6 Sn1 -96.5(17) . .
O4 W1 O6 Sn1 9.0(18) . .
O8 W1 O6 Sn1 166.8(17) . .
O33 W1 O6 Sn1 109.8(18) . .
O13 W1 O6 Sn1 94.1(17) . .
O12 W3 O7 W9 -171.9(5) . .
O10 W3 O7 W9 87.8(5) . .
O19 W3 O7 W9 -72.8(5) . .
O9 W3 O7 W9 -1.0(13) . .
O14 W3 O7 W9 2.1(4) . .
O12 W3 O7 Na6 65.9(6) . 1_545
O10 W3 O7 Na6 -34.4(6) . 1_545
O19 W3 O7 Na6 165.1(5) . 1_545
O9 W3 O7 Na6 -123.2(10) . 1_545
O14 W3 O7 Na6 -120.1(5) . 1_545
O27 W9 O11 Mn1 65.3(9) . .
O2 W9 O11 Mn1 -36.9(9) . .
O18 W9 O11 Mn1 164.7(8) . .
O7 W9 O11 Mn1 -109.0(12) . .
O14 W9 O11 Mn1 -122.0(8) . .
O7 W3 O12 Na2 148.9(7) . 2_754
O10 W3 O12 Na2 -116.7(7) . 2_754
O19 W3 O12 Na2 57.5(7) . 2_754
O9 W3 O12 Na2 -27.5(7) . 2_754
O28 W4 O16 W8 -117.2(9) . .
O33 W4 O16 W8 140.5(9) . .
O31 W4 O16 W8 41.9(17) . .
O5 W4 O16 W8 -16.9(9) . .
O13 W4 O16 W8 68.4(9) . .
O32 W7 O20 Mn1 -69.1(9) . .
O2 W7 O20 Mn1 36.2(8) . .
O21 W7 O20 Mn1 -164.2(8) . .
O26 W7 O20 Mn1 122.8(11) . .
O15 W7 O20 Mn1 122.3(8) . .
O30 W8 O21 W7 -177.7(6) . .
O22 W8 O21 W7 77.5(5) . .
O3 W8 O21 W7 -79.4(5) . .
O16 W8 O21 W7 -16.8(13) . .
O15 W8 O21 W7 -3.6(4) . .
O30 W8 O22 Sn1 51.8(7) . 2_755
O21 W8 O22 Sn1 155.7(6) . 2_755
O3 W8 O22 Sn1 -102.6(10) . 2_755
O16 W8 O22 Sn1 -47.0(7) . 2_755
O15 W8 O22 Sn1 -130.0(7) . 2_755
O29 W6 O23 Sn1 -44.3(8) . .
O18 W6 O23 Sn1 -144.6(7) . .
O17 W6 O23 Sn1 56.4(8) . .
O19 W6 O23 Sn1 125.2(9) . .
O14 W6 O23 Sn1 142.8(8) . .
O4 W1 O24 Mn1 -22(3) . 2_755
O6 W1 O24 Mn1 78(3) . 2_755
O8 W1 O24 Mn1 166(3) . 2_755
O33 W1 O24 Mn1 -111(3) . 2_755
O13 W1 O24 Mn1 -141(2) . 2_755
O26 W5 O25 Na5 40.4(8) . 2_754
O5 W5 O25 Na5 -144.5(7) . 2_754
O10 W5 O25 Na5 -53.2(7) . 2_754
O3 W5 O25 Na5 128.9(7) . 2_754
O26 W5 O25 Na4 -125.5(8) . 2_754
O5 W5 O25 Na4 49.5(8) . 2_754
O10 W5 O25 Na4 140.9(8) . 2_754
O3 W5 O25 Na4 -37.0(8) . 2_754
Na5 W5 O25 Na4 -165.9(12) 2_754 2_754
O16 W4 O28 Na2 92.2(9) . .
O33 W4 O28 Na2 -170.0(8) . .
O31 W4 O28 Na2 -80.6(9) . .
O5 W4 O28 Na2 3.2(9) . .
O13 W4 O28 Na2 -116.3(18) . .
O23 W6 O29 Na2 -131.0(7) . 1_455
O18 W6 O29 Na2 -32.4(7) . 1_455
O17 W6 O29 Na2 135.8(7) . 1_455
O19 W6 O29 Na2 53.2(7) . 1_455
O14 W6 O29 Na2 7(3) . 1_455
O20 W7 O32 Na1 4.5(13) . 1_545
O2 W7 O32 Na1 -92.7(12) . 1_545
O21 W7 O32 Na1 95.7(12) . 1_545
O26 W7 O32 Na1 -179.7(11) . 1_545
O15 W7 O32 Na1 142.9(11) . 1_545
O28 W4 O33 W1 172.6(5) . .
O16 W4 O33 W1 -83.4(5) . .
O31 W4 O33 W1 76.4(5) . .
O5 W4 O33 W1 10.3(13) . .
O13 W4 O33 W1 2.4(4) . .
Sn1 C1 C2 C3 -14.1(15) . .
Sn1 O34 C3 O35 170.5(13) . .
Na1 O34 C3 O35 -21(2) . .
Sn1 O34 C3 C2 -9.7(16) . .
Na1 O34 C3 C2 158.3(9) . .
C1 C2 C3 O35 -163.5(14) . .
C1 C2 C3 O34 17(2) . .
